[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.530 - 1.730
- Minimum stability (T80, hours): 115
- Initial efficiency (JV_default_PCE, %): 20.5
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_40514
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | MoO3 | Au
_film_thickness_nm: 250.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 105.0
_anneal_time_min: 10.0
_anneal_atmosphere: N2
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.63
_targets.T80_hours: 144
_initial.JV_default_PCE_percent: 20.5


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 400
- Initial efficiency (JV_default_PCE, %): nan
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_7611
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PEDOT:PSS | Perovskite | C60 | BCP | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: UNKNOWN
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 500
_initial.JV_default_PCE_percent: nan


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: Cs, FA
- Allowed B-site ions: Pb
- Allowed X-site ions: Br, I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.620 - 1.820
- Minimum stability (T80, hours): 64
- Initial efficiency (JV_default_PCE, %): 11.7
- Soft geometry constraints: t in [0.92, 1.02], μ in [0.51, 0.61] (target t≈0.97, μ≈0.56)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_32935
_chemical_formula_sum: Cs0.15FA0.85PbBr0.87I2.13
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | SnO2-np | Perovskite | Spiro-MeOTAD | MoOx | ITO | MgF2
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 30.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
FA 0.85
Cs 0.15
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 0.71
Br 0.29

_geometry.t_goldschmidt: 0.9717
_geometry.mu_octahedral: 0.5586

_targets.band_gap_eV: 1.72
_targets.T80_hours: 80
_initial.JV_default_PCE_percent: 11.7


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 142
- Initial efficiency (JV_default_PCE, %): 16.0
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_13992
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | SnO2-np | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 65.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 177
_initial.JV_default_PCE_percent: 16.0


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 168
- Initial efficiency (JV_default_PCE, %): 10.7
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_32156
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 60.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 210
_initial.JV_default_PCE_percent: 10.7


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 16
- Initial efficiency (JV_default_PCE, %): 14.0
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_31397
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 65.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: Yes

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 21
_initial.JV_default_PCE_percent: 14.0


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 560
- Initial efficiency (JV_default_PCE, %): 19.6
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_28650
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | SnO2-c | Perovskite | Spiro-MeOTAD | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 700
_initial.JV_default_PCE_percent: 19.6


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 424
- Initial efficiency (JV_default_PCE, %): nan
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_31628
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PEDOT:PSS | Perovskite | PCBM-60 | C60 | BCP | Ag
_film_thickness_nm: 400.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 90.0
_anneal_time_min: 10.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 531
_initial.JV_default_PCE_percent: nan


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.400 - 1.600
- Minimum stability (T80, hours): 224
- Initial efficiency (JV_default_PCE, %): 17.7
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_32280
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | PPDT2FBT | Au
_film_thickness_nm: 300.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 2.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.5
_targets.T80_hours: 280
_initial.JV_default_PCE_percent: 17.7


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: Cs, FA, MA
- Allowed B-site ions: Pb, Sn
- Allowed X-site ions: Br, I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.240 - 1.440
- Minimum stability (T80, hours): 520
- Initial efficiency (JV_default_PCE, %): 12.3
- Soft geometry constraints: t in [0.92, 1.02], μ in [0.50, 0.60] (target t≈0.97, μ≈0.55)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_2188
_chemical_formula_sum: Cs0.05FA0.79MA0.16Pb0.75Sn0.25Br0.5I2.5
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PEDOT:PSS | Perovskite | PCBM-60 | C60 | BCP | Ag
_film_thickness_nm: 450.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 10.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
FA 0.79
MA 0.16
Cs 0.05
loop_
_site B_ion occupancy
Pb 0.75
Sn 0.25
loop_
_site X_ion occupancy
I 0.8333
Br 0.1667

_geometry.t_goldschmidt: 0.9717
_geometry.mu_octahedral: 0.5498

_targets.band_gap_eV: 1.34
_targets.T80_hours: 650
_initial.JV_default_PCE_percent: 12.3


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 6
- Initial efficiency (JV_default_PCE, %): 11.9
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_25694
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | DAHI | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 60.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 7
_initial.JV_default_PCE_percent: 11.9


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 160
- Initial efficiency (JV_default_PCE, %): 17.5
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_16590
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | TPA‐ANT‐TPA | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 30.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 200
_initial.JV_default_PCE_percent: 17.5


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 4
- Initial efficiency (JV_default_PCE, %): 14.3
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_30796
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 105.0
_anneal_time_min: 60.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 6
_initial.JV_default_PCE_percent: 14.3


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 4
- Initial efficiency (JV_default_PCE, %): 15.9
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_16348
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | SnO2-np; TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 6
_initial.JV_default_PCE_percent: 15.9


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 470
- Initial efficiency (JV_default_PCE, %): 16.9
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_36413
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PTAA | MoS2 | Perovskite | PCBM-60 | PFN | Al
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: Yes

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 588
_initial.JV_default_PCE_percent: 16.9


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 320
- Initial efficiency (JV_default_PCE, %): 18.1
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_32966
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 70.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 400
_initial.JV_default_PCE_percent: 18.1


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 12
- Initial efficiency (JV_default_PCE, %): 14.4
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_37869
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: PEN | ITO | NiO-c | Perovskite | PCBM-60 | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: UNKNOWN
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 15
_initial.JV_default_PCE_percent: 14.4


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 134
- Initial efficiency (JV_default_PCE, %): 11.5
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_8448
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | DEPT-SC | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: unknown >> unknown
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 168
_initial.JV_default_PCE_percent: 11.5


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 40
- Initial efficiency (JV_default_PCE, %): 12.3
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_7887
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: -173.14999999999998
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 50
_initial.JV_default_PCE_percent: 12.3


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: FA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.380 - 1.580
- Minimum stability (T80, hours): 320
- Initial efficiency (JV_default_PCE, %): 20.1
- Soft geometry constraints: t in [0.94, 1.04], μ in [0.49, 0.59] (target t≈0.99, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_17088
_chemical_formula_sum: FAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 160.0
_anneal_time_min: 20.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
FA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9866
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.48
_targets.T80_hours: 400
_initial.JV_default_PCE_percent: 20.1


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 595
- Initial efficiency (JV_default_PCE, %): nan
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_5874
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PEDOT:PSS | Perovskite | PCBM-60 | BCP | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 80.0
_anneal_time_min: 120.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 744
_initial.JV_default_PCE_percent: nan


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 60
- Initial efficiency (JV_default_PCE, %): 17.3
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_37890
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: 300.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: UNKNOWN
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 75
_initial.JV_default_PCE_percent: 17.3


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 80
- Initial efficiency (JV_default_PCE, %): 11.5
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_1906
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 50.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 100
_initial.JV_default_PCE_percent: 11.5


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 134
- Initial efficiency (JV_default_PCE, %): 12.6
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_27127
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | Spiro-MeOTAD | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: -183.14999999999998
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 168
_initial.JV_default_PCE_percent: 12.6


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 80
- Initial efficiency (JV_default_PCE, %): 7.6
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_32110
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | NiO-np | Perovskite | PCBM-60 | BCP | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 5.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 100
_initial.JV_default_PCE_percent: 7.6


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 5
- Initial efficiency (JV_default_PCE, %): 14.8
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_41953
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Carbon-QDs | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: 320.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 60.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 6
_initial.JV_default_PCE_percent: 14.8


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.450 - 1.650
- Minimum stability (T80, hours): 576
- Initial efficiency (JV_default_PCE, %): 15.7
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_27470
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | 2F-SAM | PEDOT:PSS | Perovskite | PCBM-60 | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 80.0
_anneal_time_min: 5.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.55
_targets.T80_hours: 720
_initial.JV_default_PCE_percent: 15.7


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 2
- Initial efficiency (JV_default_PCE, %): 14.5
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_21233
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 70.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 2
_initial.JV_default_PCE_percent: 14.5


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.490 - 1.690
- Minimum stability (T80, hours): 80
- Initial efficiency (JV_default_PCE, %): 18.9
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_26371
_chemical_formula_sum: MA0.98PbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: 350.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 10.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.59
_targets.T80_hours: 100
_initial.JV_default_PCE_percent: 18.9


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 100
- Initial efficiency (JV_default_PCE, %): nan
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_30761
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PEI | ICBA | Perovskite | PTAA | MoO3 | Ag
_film_thickness_nm: 350.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 10.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 126
_initial.JV_default_PCE_percent: nan


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: Cs, FA
- Allowed B-site ions: Pb
- Allowed X-site ions: Br, I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.470 - 1.670
- Minimum stability (T80, hours): 2240
- Initial efficiency (JV_default_PCE, %): 19.9
- Soft geometry constraints: t in [0.90, 1.00], μ in [0.50, 0.60] (target t≈0.95, μ≈0.55)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_9968
_chemical_formula_sum: Cs0.25FA0.75PbBr0.3I2.7
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | NiO-c | CuGaO2-mp | Perovskite | PCBM-60 | BCP | Ag
_film_thickness_nm: 600.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 20.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
FA 0.75
Cs 0.25
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 0.9
Br 0.1

_geometry.t_goldschmidt: 0.9545
_geometry.mu_octahedral: 0.5469

_targets.band_gap_eV: 1.57
_targets.T80_hours: 2800
_initial.JV_default_PCE_percent: 19.9


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 38
- Initial efficiency (JV_default_PCE, %): 17.2
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_21316
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 15.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 48
_initial.JV_default_PCE_percent: 17.2


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.400 - 1.600
- Minimum stability (T80, hours): 576
- Initial efficiency (JV_default_PCE, %): 19.3
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_8308
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PTAA | Perovskite | PCBM-60; Sb-Carbon-nw | BCP | Au
_film_thickness_nm: 300.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 10.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.5
_targets.T80_hours: 720
_initial.JV_default_PCE_percent: 19.3


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 68
- Initial efficiency (JV_default_PCE, %): 7.9
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_9159
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PEDOT:PSS | Perovskite | PCBM-60 | ZnO-np | Al
_film_thickness_nm: 400.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 95.0
_anneal_time_min: 75.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 85
_initial.JV_default_PCE_percent: 7.9


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 273
- Initial efficiency (JV_default_PCE, %): 14.6
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_28898
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: 300.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 20.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 342
_initial.JV_default_PCE_percent: 14.6


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 320
- Initial efficiency (JV_default_PCE, %): 18.1
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_32290
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: 350.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 10.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 400
_initial.JV_default_PCE_percent: 18.1


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: FA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.380 - 1.580
- Minimum stability (T80, hours): 2
- Initial efficiency (JV_default_PCE, %): 16.5
- Soft geometry constraints: t in [0.94, 1.04], μ in [0.49, 0.59] (target t≈0.99, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_32242
_chemical_formula_sum: FAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 150.0
_anneal_time_min: 30.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
FA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9866
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.48
_targets.T80_hours: 2
_initial.JV_default_PCE_percent: 16.5


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 96
- Initial efficiency (JV_default_PCE, %): 16.6
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_17108
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: UNKNOWN
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 120
_initial.JV_default_PCE_percent: 16.6


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 272
- Initial efficiency (JV_default_PCE, %): 17.7
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_2115
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 70.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 340
_initial.JV_default_PCE_percent: 17.7


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 268
- Initial efficiency (JV_default_PCE, %): 11.6
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_17005
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | Ag:CuO-nanofibers | PEDOT:PSS | Perovskite | PCBM-60 | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 30.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 336
_initial.JV_default_PCE_percent: 11.6


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 256
- Initial efficiency (JV_default_PCE, %): 17.8
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_32288
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: 350.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 10.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 320
_initial.JV_default_PCE_percent: 17.8


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 80
- Initial efficiency (JV_default_PCE, %): 19.6
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_4830
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PTAA | Perovskite | PCBM-60 | Al
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: -173.14999999999998
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 100
_initial.JV_default_PCE_percent: 19.6


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 288
- Initial efficiency (JV_default_PCE, %): 17.0
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_7804
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | ZnO-c | ZnO-nw | Perovskite | Spiro-MeOTAD | Ag
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 70.0
_anneal_time_min: 20.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 360
_initial.JV_default_PCE_percent: 17.0


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 176
- Initial efficiency (JV_default_PCE, %): 13.3
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_26
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 10.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 220
_initial.JV_default_PCE_percent: 13.3


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 252
- Initial efficiency (JV_default_PCE, %): nan
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_31320
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | XY1 | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 60.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 315
_initial.JV_default_PCE_percent: nan


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: Cs
- Allowed B-site ions: Pb
- Allowed X-site ions: Br, I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.950 - 2.150
- Minimum stability (T80, hours): 196
- Initial efficiency (JV_default_PCE, %): 7.0
- Soft geometry constraints: t in [0.85, 0.91], μ in [0.53, 0.63] (target t≈0.86, μ≈0.58)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_14606
_chemical_formula_sum: CsPbBr2I
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | SnO2-np | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: 290.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 160.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
Cs 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
Br 0.6667
I 0.3333

_geometry.t_goldschmidt: 0.8582
_geometry.mu_octahedral: 0.5833

_targets.band_gap_eV: 2.05
_targets.T80_hours: 245
_initial.JV_default_PCE_percent: 7.0


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 96
- Initial efficiency (JV_default_PCE, %): 14.1
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_171
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: 400.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 85.0
_anneal_time_min: 60.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 120
_initial.JV_default_PCE_percent: 14.1


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 1
- Initial efficiency (JV_default_PCE, %): nan
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_31041
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 1
_initial.JV_default_PCE_percent: nan


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 320
- Initial efficiency (JV_default_PCE, %): 9.2
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_17094
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | TiO2-mp | Al2O3-mp | Perovskite | Carbon; WO3-np
_film_thickness_nm: UNKNOWN
_deposition_procedure: Drop-Infiltration
_anneal_temperature_C: 50.0
_anneal_time_min: 60.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 400
_initial.JV_default_PCE_percent: 9.2


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: FA, MA
- Allowed B-site ions: Pb
- Allowed X-site ions: Br, I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.400 - 1.600
- Minimum stability (T80, hours): 1
- Initial efficiency (JV_default_PCE, %): 18.4
- Soft geometry constraints: t in [0.93, 1.03], μ in [0.50, 0.60] (target t≈0.98, μ≈0.55)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_28305
_chemical_formula_sum: FA0.9MA0.1PbBr0.3I2.7
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PTAA | Perovskite | C60 | SnS | Ag
_film_thickness_nm: 340.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 100.0
_anneal_time_min: 15.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
FA 0.9
MA 0.1
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 0.9
Br 0.1

_geometry.t_goldschmidt: 0.9810
_geometry.mu_octahedral: 0.5469

_targets.band_gap_eV: 1.5
_targets.T80_hours: 2
_initial.JV_default_PCE_percent: 18.4


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 119
- Initial efficiency (JV_default_PCE, %): 11.8
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_19584
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | PEDOT:PSS | Perovskite | C60 | BCP | Ag
_film_thickness_nm: 550.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 70.0
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 149
_initial.JV_default_PCE_percent: 11.8


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 320
- Initial efficiency (JV_default_PCE, %): 15.0
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_19977
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: PEN | ITO | TiO2-c | PCBM-60 | Perovskite | Spiro-MeOTAD | Ag
_film_thickness_nm: 450.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 50.0
_anneal_time_min: 240.0
_anneal_atmosphere: UNKNOWN
_encapsulation: No

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 400
_initial.JV_default_PCE_percent: 15.0


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 1
- Initial efficiency (JV_default_PCE, %): 12.5
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_37811
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | ITO | CPE-K | Perovskite | PCBM-60 | Al
_film_thickness_nm: 250.0
_deposition_procedure: Spin-coating
_anneal_temperature_C: 90.0
_anneal_time_min: 60.0
_anneal_atmosphere: UNKNOWN
_encapsulation: Yes

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 0
_initial.JV_default_PCE_percent: 12.5


[User]
You are a materials design assistant. Produce a CIF-LITE block that encodes a halide perovskite candidate meeting the constraints.

Constraints:
- Allowed A-site ions: MA
- Allowed B-site ions: Pb
- Allowed X-site ions: I
- Preferred perovskite dimensionality: 3D
- Band gap window (eV): 1.500 - 1.700
- Minimum stability (T80, hours): 36
- Initial efficiency (JV_default_PCE, %): nan
- Soft geometry constraints: t in [0.86, 0.96], μ in [0.49, 0.59] (target t≈0.91, μ≈0.54)
- Notes: Prefer processing similar to exemplars. Use LONG composition strings.

Return only this block:

# CIF-LITE v1
data_id: <free text label>
_chemical_formula_sum: <LONG composition string>
_perovskite_dimension: <3D|2D|2D3D|UNKNOWN>
_stack_sequence: <free text or UNKNOWN>
_film_thickness_nm: <number or UNKNOWN>
_deposition_procedure: <spin|blade|evap|spray|inkjet|UNKNOWN>
_anneal_temperature_C: <number or UNKNOWN>
_anneal_time_min: <number or UNKNOWN>
_anneal_atmosphere: <air|N2|vacuum|solvent_vapor|UNKNOWN>
_encapsulation: <Yes|No|UNKNOWN>

loop_
_site A_ion occupancy
<A_LOOP_ROWS>
loop_
_site B_ion occupancy
<B_LOOP_ROWS>
loop_
_site X_ion occupancy
<X_LOOP_ROWS>

_targets.band_gap_eV: <PREDICTED_Eg>
_targets.T80_hours: <PREDICTED_T80>

[Assistant]
# CIF-LITE v1
data_id: PD_37220
_chemical_formula_sum: MAPbI3
_perovskite_dimension: 3D
_stack_sequence: SLG | FTO | TiO2-c | Perovskite | Spiro-MeOTAD | Au
_film_thickness_nm: UNKNOWN
_deposition_procedure: Spin-coating
_anneal_temperature_C: UNKNOWN
_anneal_time_min: UNKNOWN
_anneal_atmosphere: UNKNOWN
_encapsulation: Yes

loop_
_site A_ion occupancy
MA 1.0
loop_
_site B_ion occupancy
Pb 1.0
loop_
_site X_ion occupancy
I 1.0

_geometry.t_goldschmidt: 0.9115
_geometry.mu_octahedral: 0.5409

_targets.band_gap_eV: 1.6
_targets.T80_hours: 45
_initial.JV_default_PCE_percent: nan